This is a repository copy of Investigation of pure sliding and sliding/rolling contacts in a
DLC/Cast iron system when lubricated in oils containing MoDTC-Type friction modifier.
White Rose Research Online URL for this paper:
Version: Accepted Version
Al-Jeboori, Y, Kosarieh, S orcid.org/0000-0002-0210-7165, Morina, A
orcid.org/0000-0001-8868-2664 et al. (1 more author) (2018) Investigation of pure sliding
and sliding/rolling contacts in a DLC/Cast iron system when lubricated in oils containing
MoDTC-Type friction modifier. Tribology International, 122. pp. 23-37. ISSN 0301-679X
© 2018 Elsevier Ltd. This manuscript version is made available under the CC-BY-NC-ND
4.0 license http://creativecommons.org/licenses/by-nc-nd/4.0/
This article is distributed under the terms of the Creative Commons Attribution-NonCommercial-NoDerivs (CC BY-NC-ND) licence. This licence only allows you to download this work and share it with others as long as you credit the authors, but you can’t change the article in any way or use it commercially. More
information and the full terms of the licence here: https://creativecommons.org/licenses/
If you consider content in White Rose Research Online to be in breach of UK law, please notify us by
Investigation of Pure Sliding and Sliding/Rolling Contacts in a DLC/Cast
Iron System Using MoDTC-Type Friction Modifier
, Shahriar Kosarieha
, Ardian Morinaa
, Anne Nevillea
aInstitute of Functional Surfaces (iFS), School of Mechanical Engineering, University of Leeds, LS2 9JT, UK
bMechanical Department, Design Division, State Company for Oil Projects (SCOP), Ministry of Oil, Iraq
Diamond-like carbon (DLC)/cast iron (CI) systems have been widely investigated due to their important
application in engine components such as cylinders, pistons and more specifically for the cam/follower
interface. The pure sliding contact of the DLC/CI system has traditionally been the focus of research;
consequently less is understood about sliding/rolling contact systems. In addition, the tribological and
tribochemical characteristics of the Molybdenum Dialkyl Dithiocarbamate (MoDTC) as a lubricant
additive in such sliding/rolling contacts are not fully understood.
In this study, a Mini Traction Machine (MTM) was used to run the experiments using alloy steel balls
coated with 15 atomic percent (at. %) hydrogenated DLC (a-C: 15H) rubbing against uncoated cast iron
discs. Results showed that the sliding/rolling ratio affects friction, wear and tribochemistry in CI/DLC
systems; pure sliding enhances MoDTC activation. MoDTC decomposes to form MoS2, FeMoO4and
not MoO3. In addition, it was observed that MoS2/FeMoO4ratio depends on test conditions and affects
to the friction performance.
Keywords:Sliding/Rolling, Pure Sliding, DLC/Cast Iron, MoDTC.
*Corresponding author. Tel.:+441133438000, E-mail address: email@example.com
Due to the importance of reducing emissions and improving fuel economy, there has already been a
lot of effort by different scientists in developing new lubricants or/and alternative additives without
compromising friction and wear performance of the lubricant. For example, the use of hybrid
nanomaterials as nano-lubricant additives can reduce frictional power losses in automotive engines and
can lead to an improvement in the efﬁciency of engines and fuel economy . Results of a wide
spectrum of nanoscale additives have been reported in the tribology literature and a review is beyond
the scope of this paper. It is important to note that the optimisation of the frictional and durability of a
tribological contact relies upon the understanding of the surface/lubricant interactions and with
replacements to conventional steel now being common place, a major priority is to understand how
some of the conventional friction modifiers (like Molybdenum Dialkyl Dithiocarbamate (MoDTC))
interact with conventional (steel) and less conventional (DLC) surfaces. The heavy elements can be
surface properties then there is potential to optimise formulations. In conventional steel/steel contacts,
MoDTC has been shown to produce Mo-S compounds which in turn provide low friction under
boundary lubrication by forming MoS2low friction sheets on the tribological contact [2-4]. In addition,
MoDTC additive was reported to produce MoO3compounds in the tribofilm [3, 5]. Moreover,the iron (II) molybdate (FeMoO4) is being reportedas a product of MoDTC decomposition [2, 4]. On the other
hand, different studies have been focused to evaluate the interactions between MoDTC and ZDDP.
Martinet al.  suggested a two-step reaction which occurs in the presence of MoDTC/ZDDP. The first reaction is between phosphate and iron oxide while the second reaction is between the nascent iron
surface and a sulphide species. Essentially, it was found that Zinc DialkyIDithioPhosphate (ZDDP)
might promote MoS2formation from MoDTC sheets. In addition, it was reported that MoDTC is more
effective when used together with ZDDP and the combination of both was reported to provide better
tribological performance (i.e., less friction and wear) .
DLC coatings have attracted a lot of interest as a surface engineering solution for engine components
by offering outstanding friction properties, high wear resistance, high electrical resistance, high
corrosion resistance, high hardness and excellent running-in properties. Many researchers have
evaluated the behaviour of DLC coatings under the presence of additives including MoDTC. It is
generally shown that DLC coatings offer friction reduction by forming MoDTC derived MoS2sheets
on DLC surfaces [8, 9]. The hydrogenated DLC films are considered to provide the counterbody with
a carbon layer, where these layers are responsible to reduce friction on DLC surfaces . However,
recently, it has been reported [11-14] that DLC coatings wear faster in the presence of MoDTC when
rubbed against a ferrous counterpart. Kosariehet al., showed that high concentration of MoDTC promoted wear of the hydrogenated DLC coating in oils without ZDDP but this wear was mitigated by
the addition of ZDDP. Based on the published literature [3, 11-19], it appears that MoDTC-derived
products are key to this detrimental effect and that ZDDP might hinder the MoDTC potency in giving
high wear to DLC in the DLC/ferrous combinations . MoDTC-induced wear of the DLC coatings
was only observed when the DLC was rubbed against a ferrous counterpart [3, 14]. That was attributed
to the formation of molybdenum-containing compounds in the presence of ferrous counterparts leading
to oxidation and accelerated wear of the DLC coating .
Sliding and rolling contacts are widely presented in different mechanical components such as cams,
gears and roller bearings. The combination of sliding/rolling motion can cause lubrication difficulties,
high loads/applied stresses and film thickness variation. As a result, wear and plastic deformation can
be observed which may lead to failure of the components. In the literature, however, most of the
previous works have tended to focus mainly on pure sliding contacts, probably due to the fact that the
pure sliding contacts are generally observed to be more severe than sliding/rolling contacts . It
in mechanical components as they mostly experience the combination of both motions (i.e. pure sliding
and sliding/rolling). Thus, it is essential to investigate both the sliding and sliding/rolling contacts and
to compare their tribological and tribochemical performance under mixed-boundary lubrication
regimes. In general, the correlation between the sliding/rolling ratio (SRR) and the
tribological/tribochemical performance was reported previously [2, 21-26]. For the friction
performance, it has been generally shown that the increase of the sliding/rolling ratio (SRR) causes an
increase of friction. For example, increasing sliding/rolling ratio from 100% to 200% increases
boundary friction . In addition, it was reported that elastohydrodynamic friction was increased when
increasing sliding/rolling ratio from 10% to 50% . Vengudusamy et al. studied the friction behaviour of five gear oils at three different sliding/rolling ratios, 30%, 50% and 200%. They reported
that the increase of the boundary friction was significant when SRR was 200% (i.e. pure sliding) while
it was marginal between 30% and 50%.
The tribochemical reaction is typically attributed to the formation of a tribofilm layer. Tribofilms
work as a third body between the interacting surfaces which in turn provide an ultralow friction and a
low wear rate. The chemical composition of the tribofilms and/or tribofilm evolution are understood to
vary with changing contact type (e.g. pure sliding contact + sliding/rolling contact). However, the
understanding of the tribofilm formation due to changes in the tribological system, such as changing
the type of contact (i.e. implying different SRR values) has not been given special attention. In the
literature, the effect of sliding/rolling ratio on ZDDP tribofilm formation was previously investigated
. In addition, the tribofilm generation for a base oil and a fully formulated oil under the influence
of sliding/rolling ratio was also examined . Moreover, Khaemba et al.  studied the role of sliding/rolling ratio and surface roughness on the decomposition of MoDTC in a steel/steel system.
However, in a DLC/CI system, there is still limited understanding about how sliding/rolling ratio affects
tribofilm build-up when using lubricants containing MoDTC additive. With this understanding, the
main aim of the work is to study and compare the tribological behaviour of two types of DLC/CI
contacts (pure sliding contact + sliding/rolling contact) under mixed-boundary lubrication regimes. The
second aim is to investigate the variation of tribofilm compositions in both contacts. This was achieved
in a DLC/CI system lubricated in a fully formulated oil / base oil containing MoDTC.
2. Experimental procedure
The mini-traction machine (MTM) was used to produce tribofilms under mixed-boundary
lubrication conditions, where a 19.05 mm diameter ball was loaded and rubbed against a 46 mm
diameter disc and both were submerged in the lubricant. The samples were cleaned ultrasonically prior
to the start of the test using acetone for at least 15 minutes. Further, the samples were wiped with a
cotton bud soaked in isopropanol. Lastly, an airbrush with isopropanol was used to clean the samples
Stribeck curve tests. Durability tests are used to observe the stability of the DLC/CI system over a period
of time under the boundary lubrication regime. Stribeck curve tests are used to evaluate the friction
properties of the DLC/CI system under mixed-boundary lubrication regimes. The test conditions
employed in this study were: applied load = 33.85 N, corresponding to a contact pressure of 0.75 GPa;
entrainment speed = 100 mm/s; temperature = 100 °C; sliding/rolling ratio = 50% and 200%;
running-in duration = 30 mrunning-ins; test duration = 6 hrs. The entrarunning-inment speed with respect to the contactrunning-ing
surfaces was represented as (ub + ud)/2, where ubis the speed of the ball while ud is the speed of the
disc. The sliding/rolling ratio was represented as the ratio of sliding speed ub- ud to entrainment speed. However, SRR= 50% represents the sliding/rolling contact (this ratio is selected as a standard
slipping ratio) while SRR = 200% represents the pure sliding contact (the ball was held stationary and
the disc was allowed to rotate). The durability test was calculated at 100 mm/s during the whole test
duration (6.5 hrs) which is in the boundary lubrication regime. The Stribeck curve test was obtained by
measuring friction over a range of entrainment speeds ranging from low to high speeds, 5 to 2000 mm/s.
Film thickness develops with increasing entrainment speed, progressing from boundary lubrication
regime at low speed through to mixed lubrication regime at high speed.
In this study, the White Light Interferometer (Bruker NPFLEX) was used to characterize the wear
of the DLC coated balls and Cast Iron (CI) disks. Therefore, before these analyses, in order to remove
any physisorbed tribofilm formed on the wear scar, a droplet of ethylenediaminetetraacetic acid (EDTA)
was used (by the method described in ) to remove the tribofilm from the analysed wear track.
However, the droplet was removed with a cotton bud and the samples were cleaned with an airbrush
filled with isopropanol. This was done to avoid any misleading wear measurements due to the
transparent characteristics of the formed tribofilm . Two-dimensional and three-dimensional images
for the wear track were taken, and the average wear depth of different sections inside the wear track
.Balls were made of alloy steel 16MnCr5 and discs were made of cast iron (CI). Balls
were coated by commercial DLC coatings which contained 15 at. % hydrogen (a-C: 15H). The detailed
physical properties of the DLC coating, balls and discs are given in Table 1. The lubricants used in the
experiments are Group III mineral base oil and fully formulated oil, grade 5W30. All the oils were
commercial and supplied by Total. Initially, several concentrations of MoDTC ranging from 0.1wt %
to 0.5 wt % were blended with the lubricants used in this study. However, considering the test duration,
it was found that the effect of these low concentrations on friction reduction was insignificant and
therefore we could not discriminate between different oil formulations with regards to friction
performance. For this reason, 1 wt% concentration of MoDTC was used in this work. With respect to
lubricants containing ZDDP, the lubricant used was provided by Total with 1 wt% concentration of
ZDDP. The detailed chemistry of oils cannot be shown due to confidentiality, but the key additive
lubricant oil samples is shown in Fig.1. Lambda ratio and the film thickness were calculated using
Equations (1) and (2) respectively .
= 3.63 ´
. ´ . ´ . . (1) = = = + (2)
Where is the minimum film thickness, is the reduced radius of curvature, is the entraining
surface velocity, is the dynamic viscosity of the lubricant at atmospheric pressure, is the
viscosity-pressure coefficient, is the normal load, ´ is the reduced Young’s modulus, is the Root Mean
Square (RMS) roughness of the two surfaces in contact, is the surface roughness of the DLC coating
and the is the surface roughness of the CI disc. The calculated Lambda ratio showed that the
operating regime was boundary lubrication ( = 0.1) for the durability test and mixed-boundary
lubrication (ranging from =0.1 at low speed to = 1.2 at high speed) for the Stribeck curve tests. For
BO and O1, however, the calculated Lambda ratio was not exceeding 0.9 at high speed implying a
boundary lubrication regime throughout the Stribeck curve tests for these oils.
Table 1.Physical properties of balls, discs and DLC coating
Balls Discs DLC coating
Specification 16MnCr5 Steela EN-GIL-250 Grey cast irona a-C: 15Hb
Hardness 7.453-7.846 GPa 2.256-2.354 GPa 20-25 GPa
Roughness, Rq 0.02-0.05 m 0.08-0.11 m 0.02-0.05 m
modulus 207 GPa 110 GPa 160-200 GPa
C 0.16, Si 0.20%, Mn 1.11%, P 0.011%, S
0.026%, Ni 0.07%, Cr 0.90%, Mo 0.01%, Cu
0.14%, Sn 0.10%, Al 0.022%, N 0.0101%
C 3.34%, Si 2.40%, Mn 0.49%, P 0.081%,
S 0.060%, Mg 0.001% 1.5-3 m
aBalls and discs provided by PCS instruments, UK.
Table 2.Lubricant components
Fig. 1.Photograph showing six representative occurrence oil samples
3. Surface analysis
Scanning Electron Microscopy (SEM) was used to examine the worn ball/disk surfaces and to
investigate the durability of the coatings employed. An Oxford instrumented EDX with scan size of 80
mm2was incorporated into the SEM device (Zeiss EVO MA15 variable pressure) to provide elemental
composition of the different regions on the samples. In this work, Energy-Dispersive X-ray (EDX)
spectra of the balls and the discs were obtained from inside the wear track. Raman spectroscopy has
been widely used to determine the structure/composition of the tribofilms generated in a tribocontact.
A Renishaw inViaTMRaman spectrometer with 488 nm wavelength and 10% power filter was used to
observe the structural modifications inside the wear track of the inserts. To support the results from
EDX and Raman spectroscopy, X-ray Photoelectron Spectroscopy (XPS) analysis was also carried out
in this study. This technique allows the tribofilms chemistry to a depth of approximately 5 nm to be
Annotations Oil formulation
BO Base oil B
O1 Base oil B + 1 wt% MoDTC
O2 Fully formulated oil B (free of ZDDP/MoDTC)
O3 Fully formulated oil B (free of MoDTC) + 1 wt% ZDDP
O4 Fully formulated oil B (free of ZDDP) + 1 wt % MoDTC
determined. Before using XPS analysis, all samples were cleaned using n-heptane to remove residual
oil and contaminants. The electrons were excited with a micro focused monochromatic aluminium
K-alpha X-ray source of 1486.6eV. A handbook of XPS was used to identify the chemical species at the
respective binding energies . The XPS curves were processed using the CasaXPS software. The
position of the major component of the C1s peak (284.8 eV) was considered as the reference for charge
4.1. Friction results
4.1.1. The correlation between SRR and friction
Initially, the MTM durability test is essential to identify the stability of the system through a
particular period. Figure 2 shows friction coefficient values during the whole test duration at 50% SRR
and 200% SRR values. All MTM tests lasted for 6.5 hrs and were started with 30 minutes running-in
followed by a Stribeck curve test for 1-2 minutes then a durability test for two hours. This procedure,
except the running-in period, is repeated twice. The fluctuation in the data at 1800 s, 9000 s and 16200
s is where the Stribeck (speed-scanning) tests were done. In general, all oils followed the same trend
with time but there were quite clear fluctuations when SRR was 200% and this resulted from the severe
conditions of the test. The steady state friction, under boundary lubrication, was presented as the average
friction values of the last hour of each test. Accordingly, Fig. 3 shows the average of coefficients of friction for all oils at 50% SRR and 200% SRR. It can be seen that no systematic trend of friction
Fig. 2.Friction coefficients as a function of time: (a) at 50%SRR and (b) 200%SRR
4.1.2. The correlation between SRR and Stribeck curve evaluation
The Stribeck curve evaluation gives an indication of the tribofilm build-up and the time to reach
steady state conditions. Fig. 4 and 5 show Stribeck curves for each oil as a function of time and mean
speed under the sliding/rolling (50% SRR) and the pure sliding (200% SRR) conditions. Asystematic
trend of friction coefficient was seen for both SRR values over time.For example, comparing the first 30 minutes to the following 2 hrs of the tests, friction was generally higher at 50% SRR (i.e.
sliding/rolling contact) than 200% SRR (i.e. pure sliding contact) for oils containing MoDTC. This
suggests a slower build-up of tribofilms in sliding/rolling contacts compared to a pure sliding contact.
For the lubricants with no MoDTC (BO, O2, O3), the change in friction over time was not significant
at 200% SRR. However, at 50% SRR, for O2, a considerable change in friction over time was seen
suggesting tribofilm evolution over a much longer timeframe.
In order to have a better picture of the SRR effect on the tribological behaviour of the lubricants
under the boundary lubrication regime, friction coefficients for each oil at mean speed = 10 mm/s
represents the boundary lubrication regime were plotted (see Fig. 6) at 50% SRR and 200%. From Fig.
6, it can be seen that SRR can play an important role in the frictional behaviour for the lubricants
containing MoDTC (i.e. O1, O4 and O5). In particular, pure sliding contact enhanced the activation of
MoDTC over time. It is also interesting to note that the lubricant with ZDDP only (i.e. O3) was not
affected by different SRR values and the friction responses were comparable over time. The observed
reduction or difference in friction between both contacts was expected to be influenced by change in
surface roughness over time in addition to changes in surface chemistry. The surface roughness for balls
and discs at the end of each test was investigated, as shown in Table 3. Comparing the surface roughness
after the test to the initial roughness (see Table 1), rougher surfaces were observed for both the discs
and the balls after the tests. Nevertheless, friction reduction was reported over time for most oils. The
tribological performance is more controlled by the contact type and the tribofilm formed on the ball/disc
tribopair rather than the surface roughness. This means that the Lambda ratio progressively decreases
Fig. 6.Friction coefficients for (a) BO, (b) O1, (c) O2, (d) O3, (e) O4 and (f) O5 at mean speed = 10 mm/s
Table 3:Range of surface roughness for balls and discs at the end of each test
Roughness, Rq ( m)
50% SRR 200% SRR
Disc Ball Disc Ball
BO 0.22-0.36 0.05-0.31 0.13-0.12 0.09-0.20
O1: BO+MoDTC 0.11-0.29 0.10-0.15 0.15-0.20 0.09-0.31
O2: FF(MODTC/ZDDP-free) 0.19-0.21 0.03-0.16 0.20-0.22 0.09-0.32
O3: FF+ZDDP (MoDTC-free) 0.14-0.15 0.11-0.13 0.12-0.30 0.07-0.11
O4: FF+MoDTC(ZDDP-free) 0.13-0.27 0.04-0.13 0.23-0.37 0.03-0.11
O5: FF+(MoDTC+ZDDP) 0.11-0.17 0.12-0.16 0.13-0.20 0.09-0.33
4.1.3. Range of friction values in the boundary lubrication regime
Table 4 shows how the addition of MoDTC affects steady state friction values for the DLC/CI system
when lubricated in base oil, fully formulated (FF) oil without ZDDP and fully formulated oil with ZDDP
under boundary lubrication regime. From Table 4, it is apparent that regardless of the type of contact,
the addition of MoDTC to the oil formulations always improved the frictional properties of the DLC/CI
system. In the case of fully formulated oil B containing ZDDP (i.e. O3 and O5), it can be seen that the
positive effect of MoDTC on reducing friction was more pronounced for the pure sliding contact.
The range of friction values ( ) is defined as the difference between the highest friction value (i.e.
at the start of the test) for each test duration and the lowest friction value under the boundary lubrication
regime (i.e. when <1). values for all lubricants and for different time intervals throughout the tests
are plotted in Fig. 7. From Fig. 7 (a), at 50% SRR, MoDTC offered the highest friction reduction for
the first 2 hrs for O1 and O5 while the highest friction reduction was observed for O4 when the test ran
for 4 hrs. Fig. 7 (b), at 200% SRR, the effect of MoDTC on friction reduction was considerable during
the running-in period (i.e. initial 30 minutes). Interestingly, the range of friction values for the lubricant
with ZDDP alone was quite constant and was not affected over time. It is clear that friction coefficient
values were observed to vary quite considerably for most of the lubricants. This is quite an important
finding as most of the modelling works assume a constant value for ( ) across the boundary lubrication
regime . In practice, however, friction values may vary due to the changes in surface physical,
chemical and mechanical properties. In addition, surface topography experiences significant
Table 4:Average of steady state friction in boundary lubrication at the last hour of each test
Average of steady state friction coefficients when <1
50% SRR 200% SRR
Without MoDTC With MoDTC Without MoDTC With MoDTC
BO 0.08 0.05 0.09 0.06
FF (free of ZDDP) 0.08 0.07 0.09 0.06
FF + ZDDP 0.1 0.06 0.1 0.05
Fig. 7.Range of friction values at <1 for all oils: (a) at 50% SRR and (b) at 200% SRR
4.2. Wear results
Post-test physical observation of DLC balls by optical microscope indicated a very shallow wear scar on all balls irrespective of the oil formulation which made the quantitative analysis of the wear scar
on all DLC balls a challenge. In order to quantify the wear depth of the coated balls and CI disks, White Light Interferometer (WLI) was used. Representative images of the wear track that formed on both the CI disk and the DLC coated ball are shown in Fig. 8. Furthermore, wear depths for both the discs and
the balls were evaluated and shown in Fig. 9. It is important to observe that no lubricants show extremely high wear on DLC coating. In addition,the uncoated cast iron discs exhibited more wear than
the DLCcoated balls, as expected, because of the large difference in hardness.This is in line with other published literature where they found lower wear of the DLC coated balls as compared to the uncoated
disk [14, 31, 32].
0 0.01 0.02 0.03 0.04 0.05 0.06 0.07 0.08 0.09 0.1
BO O1 O2 O3 O4 O5 BO O1 O2 O3 O4 O5
30 Minutes 2 Hours 4 Hours 6 Hours
Fig. 8.Representative interferometer images of the wear track that formed on: (a) uncoated cast iron disc and (b) DLC coated ball
Fig. 9.Average of wear depths that formed on: (a) uncoated cast iron discs and (b) DLC coated balls (note different wear depth scales)
4.3. Chemical analysis of tribofilm
From Fig. 10, SEM micrographs of the CI discs revealed that interactions took place among the oil
formulation, type of contact, the disc surface and the DLC ball surface. However, the DLC balls were
not clearly identified by SEM and the micrographs were seen to be similar under the effect of contact
type and oil formulation.
EDX semi-quantification of CI discs and DLC balls (for Mo, Zn, P and S elements) is presented in
Fig. 11. Essentially, the chemical composition of the tribofilms was found to vary with changing the type of contact and the oil formulation. Generally, greater Mo, Zn, S and P was reported on CI discs than DLC balls. Thisreveals that the tribofilm formed on the CI discs was thicker than the tribofilms
formed on the DLC balls. Similar findings were seen by Raman spectroscopy and X-ray photoelectron
Comparing sliding/rolling contact to pure sliding contact, the CI disk lubricated in O1 showed similar characteristics under both contacts. Nevertheless, low friction and good wear was observed
under pure sliding contact. This clearly confirms that the tribological performance was not only controlled by the tribofilm formed on the surface but also by the contact type. Although quite similar
amounts of Mo were detected on the CI discs (lubricated in O4) under both contacts, a clear reduction in friction was reported under pure sliding contact. For the DLC balls lubricated in O1, O4 and O5, only
Fig. 10.SEM micrographs of CI disks at end of test
Delamination across the wear scar
Mild wear Severe delamination across the
Polishing wear No evidence of wear
Wear debris Polishing wear
Wear debris Polishing wear
Pure sliding contact
Fig. 11.EDX semi-quantification of regions inside the wear track balls under both contacts on: (a) uncoated cast iron discs and (b) DLC balls (note different wt% scales)
4.3.2. Raman spectroscopy
Based on the literature,the expected shift in Raman spectroscopy for molybdenum disulfide (MoS2)
is reported at 383-410 cm-1, molybdenum trioxide (MoO
3) at 828-951 cm-1, carbon (C) at 1366-1596
(Fe2O3) at 120-310 cm-1and magnetite (Fe3O4) at 670-680 cm-1 [4, 33-35].Raman spectra obtained from the CI discs under both contacts is shown in Fig. 12.Raman spectra are plotted
on the same scale and have been shifted vertically for clarification purposes.For the CI disks lubricated
with MoDTC additive (i.e. O1, O4 and O5), the Raman spectra under sliding/rolling contact indicated the presence of MoS2in the range of (380-413 cm-1).For all lubricants containing MoDTC, MoO3was
molybdate FeMoO4[2, 4]. The iron molybdateis clearly detected when using O1 while there was little presence of FeMoO4when using O4 and O5. Due to the graphite normally present in the microstructure
of the cast iron, peaks due to the formation of graphitic carbon are observed on the CI disc surface. The
G and D peaks were around 1595 cm-1and 1367 cm-1respectively. However, carbon peaks were not
clearly pronounced when using O1, O2 and O5 as compared to the CI disks lubricated in BO, O3 and
O4. Fe2O3peaks (197-299 cm-1) were observed for BO, O1, O4 and O5. In addition, Fe3O4was clearly
detected in the range of (671-685 cm-1) when using BO, O1, O3 and O4. In contrast, there was no
presence of Fe2O3and Fe3O4for all lubricants under pure sliding contact.
Figure 13 shows the intensity of MoS2and FeMoO4for all oils containing MoDTC (i.e. O1, O4 and
O5) under both contacts. Comparing pure sliding contact to sliding/rolling contact, higher intensity of
MoS2(385-411 cm-1) was clearly observed. This is in agreement with the friction results (i.e. lower
friction was reported for O1, O4 and O5 under pure sliding contact as compared to sliding/rolling
contact). In addition, for pure sliding contact, FeMoO4(925 cm-1)was only detected when using O1.
Raman peaks due to the presence of carbon (1595 cm-1-1367 cm-1) were not observed when using O4
On the other hand,for both contacts and for all lubricants used in this study, Raman spectra for the DLC balls have shown similar characteristics or film structures (i.e. no structural modifications have occurred), as shown in Fig. 14.Carbon peaks were the only peaks that clearly indicated on the DLC
ball surface. The G and D peaks were around 1550 cm-1and 1370 cm-1respectively. For the G peak,
under both contacts, the Raman spectra showed no difference in the value of the full-width at
half-maximum (FWHM) and the value of the ratio HD/HG. This might suggest that no structural modification
of the DLC balls has happened after 6.5 hrs test duration. However, based on EDX results, Mo was
detected in most DLC ballslubricated with MoDTC additive (i.e. O1, O4 and O5). Nevertheless, no
MoS2and/or MoOxpeaks were observed on the DLC balls.This could either be due to a low amount
of tribofilm formed or the surface sensitivity of the Raman Spectroscopy. Therefore, to confirm previous findings, all samples were examined using X-ray photoelectron spectroscopy (XPS).Details
Fig. 12.Raman spectroscopy for the CI discs under: (a) sliding/rolling contact, (b) pure sliding contact
Fig. 14.Raman spectroscopy for the DLC coated balls under: (a) sliding/rolling contact, (d) pure sliding contact
From previous XPS analyses, tribofilms of lubricants containing MoDTC showed Mo 3d peaks at
229, 232.3 and 235 eV [36, 37]. The tribofilms of lubricants containing MoDTC were thought to be
composed of MoO3because of the presence of Mo 3d5/2peak at 232.3 eV. The Mo 3d5/2peak for FeMoO4
is also reported at 232.3 eV [38, 39]. As molybdenum in MoO3and FeMoO4have the same oxidation
state (+6), it is impossible to distinguish the two compounds (i.e. MoO3or FeMoO4) from XPS analysis
. However, Raman spectroscopy is capable of clearly distinguishing molybdenum species, even if
these species have the same oxidation state. Thus, MoO3or FeMoO4peaks were clearly distinguished
from Raman analysis [40, 41]. In this work, Raman peaks belonging to FeMoO4were clearly observed
but MoO3 peaks were not detected at all. Therefore, for the XPS results, it was believed that the Mo
3d5/2peaks are due to the presence of FeMoO4and not MoO3.
For both contacts, the fitted Mo 3d peaks obtained from the CI discs lubricated in oils containing
MoDTC (i.e. O1, O4 and O5) are shown in Fig. 15. Unlike Raman results, it can be seen that regardless
of the contact type, FeMoO4and MoS2were all identified in the tribofilms formed on the CI disks. For
all lubricants, the MoS2/FeMoO4ratio was higher under pure sliding contact compared to sliding/rolling
contact. It is also evident that the quantity of Mo, as detected by the Mo 3d peak on the CI disk under
which were found to be the lowest when using O5. From Fig. 15, it is also evident that FeMoO4was
not detected on the disc before test, this confirms that FeMoO4come from the tribofilm, not the original
surface. For both contacts, the XPS spectra of ZDDP derived species (Zn 2p and P 2p) formed on the
CI disks using O3 and O5 are shown in Fig. 16. It can be seen that Zn-phosphate and ZnS/ZnO species
were formed on the CI discs under both contacts.
Unlike the Raman spectra on the DLC balls, XPS spectra showed that FeMoO4and MoS2 were
generally observed on the tribofilms formed on the DLC balls. For both contacts, the fitted Mo 3d peaks
obtained from the DLC balls lubricated in oils containing MoDTC (i.e. O1, O4 and O5) are shown in
Fig. 17. It was evident that the intensity of FeMoO4 was higher under sliding/rolling contact as
compared with the pure sliding contact. For O5, the amount of Mo 3d detected on the tribofilm formed
on the DLC was higher under pure sliding contact compared to the sliding/rolling contact. This result
validates the friction results obtained by the DLC ball under sliding/rolling contact. For both contacts,
the XPS spectra of ZDDP derived species (Zn 2p and P 2p) formed on the DLC balls using O3 and O5
is shown in Fig. 18. It can be seen that the formation of the phosphate film was not affected by the
presence of MoDTC. For O5, the amount of Zn 2p and P 2p detected on the DLC ball was slightly
higher under pure sliding contact compared to the sliding/rolling contact. The obtained results could
justify the wear performance of the DLC ball under pure sliding contact. For both contacts, the fully
formulated lubricant (O5), which contains MoDTC and ZDDP, has shown the best tribological
performance (i.e. lower friction and wear) of all the tested lubricants. XPS depth profiling for O5 only
for both contacts is shown in Fig. 19. For clarification purposes, Fig.19 is plotted on different scales.
For both contacts, the tribofilm formed on the CI discs was relatively thicker than the tribofilms formed
on the DLC balls.
Fig. 16.XPS spectra of the discs lubricated with ZDDP: (a) Zn 2p under sliding/rolling contact, (b) Zn 2p under pure sliding contact, (c) P 2p under sliding/rolling contact, (d) P 2p under pure sliding contact
Fig. 19.Depth profiles of the discs and balls lubricated in O5: (a) Fe, (b) Zn, (c) P, (d) Mo (note different at. %
5.1. Effect of oil formulation and contact type on Stribeck curve evaluation
For 50% SRR (see Fig. 4), it is clear that most of the lubricants showed a low friction coefficient of
about 0.04 at high entrainment speed, characteristic of the mixed lubrication regime. The lubricant film
provides partial separation; the contact load is shared between the contacting asperities and the film as
a result of some mechanical interactions [42, 43]. At low entrainment speed, however, all of the
lubricants showed higher friction, characteristic of the boundary lubrication regime, where extensive
interactions occur and behaviour is characterised by the formation and removal of thin films of
molecular proportions called tribofilms . In the absence of additives, BO exhibited fluctuating
friction values over varying entrainment speeds. MoDTC has no clear effect on friction reduction for
completely formed, as reported by Grossiordet al. and Raiet al.. BO gave the lowest friction among all other oil formulations for speeds ranging from 5 to 330 mm/s. Friction values were slightly
reduced after 2 hrs of rubbing for all oil formulations and the reduction in friction was particularly
significant for O5, probably due to a synergy between MoDTC and ZDDP. This is in line with the
literature where MoDTC was found to be more effective when used together with the ZDDP and the
combination of both was reported to significantly improve the tribological performance . BO still
exhibited fluctuating friction values after 2 hrs of rubbing, likely due to the absence of additives. Early
work [36, 47, 48] has shown that the MoDTC additive readily forms MoS2sheets under mixed-boundary
lubrication regimes offering low friction on the tribological contacts. As a result, MoDTC played an
essential role in reducing friction after 4 hrs of rubbing; O1 and O5 showed a higher friction reduction
when compared to the rest of the oil formulations. Stable friction was reported after 6 hrs of rubbing.
O3 gave the highest friction among all other oil formulations for speeds ranging from 5 to 530 mm/s.
This is in line with the literature where tribofilms formed by ZDDP showed higher friction performance
. ZDDP increases friction when added to the lubricant due to the formation of pad-like tribofilm.
For pure sliding (200% SRR) contact (see Fig. 5), it is apparent that the effect of MoDTC and ZDDP
in the first 30 minutes of rubbing is negligible. This is mainly because tribofilms of both additives need
sufficient time to form on the surface. The lowest friction was about 0.03 which resulted from O2 and
is characteristic of the mixed lubrication regime. One similarity between base oil and ZDDP alone was
that BO and O3 gave the highest friction of about 0.1, probably due to the absence of additives in BO
and the presence of ZDDP in O3. The effect of both MoDTC and ZDDP additives was more pronounced
after 2 hrs of rubbing which led to a lower friction response. For this contact (i.e. pure sliding) O3 still
showed the highest friction which was likely due to the presence of ZDDP.
5.2. Effect of MoDTC on wear
From Fig. 9-a, cast iron discs showed relatively high wear when lubricated with O1 and O4 (i.e.
MoDTC alone), suggesting a negative effect of MoDTC in increasing wear of a ferrous counterpart rubbed against a DLC coating . In line with the literature, the interaction between MoDTC and ZDDP at O5 gave the lowest wear to the CI disk . ZDDP in O3, as expected, played a key role in
reducing wear of the CI disk.In the absenceof ZDDP (i.e. BO, O1, O2 and O4),sliding/rollingcontact
appears to exhibit more wear than pure sliding contact on the CI disks, suggesting that the wear
reduction is not only controlled by the oil chemistry but also by the type of contact. That could be attributed to a slower build-up of tribofilms for the sliding/rolling contact compared to the pure sliding
contact. Some previous works [3, 11-13] have reported high wear of DLC coatings in presence of MoDTC. In contrast, very limited studies showed reduction in wear of a DLC coating when lubricated
tests in DLC/DLC contact and a few tests in DLC/steel contacts. In this study, from Fig. 9-b,it is clear that no lubricants show extremely high wear on the DLC coating. For the DLC balls lubricated with
MoDTC additive, a ferrous surface (i.e. CI disc) was expected to help in increasing the wear of the DLC
coating if iron oxide particles are presented in the DLC/cast iron interface . However, in the absence
of ZDDP, DLC coated balls showed quite low wear when MoDTC was present in the oil formulation
(i.e. O1 and O4). Tunget al. studied DLC/cast iron contacts and also reported that MoDTC reduces wear of a DLC coating in a formulated engine oil. There is however no evidence whether the formulated
lubricants in Tunget al. contained ZDDP or not, as this anti wear additive could supress the effect of MoDTC on promoting wear of DLC coatings . Comparing O3 with O2, the presence ofZDDP
in the oil formulation reduced the wear of the DLC balls  but the wear reduction was not considerable. Sliding/rolling contacts for all formulated lubricants (except for BO and O1) exhibit
relatively higher wear than pure sliding contact on the DLC coated balls.This suggests that the pure sliding contact probably facilitated the build-up of tribofilms on the interface which in turn resulted in
an enhanced lubrication and thus reduced wear of the DLC balls.
5.3. Effect of contact type on tribofilm evolution
The XPS analyses showed that a tribofilm on both tribopairs is formed under both contacts. Unlike
recent work , it was found that the SRR values used in this study did affect the surface chemistry
(i.e. tribofilm build-up was seen to be influenced by the change in SRR). Table 5 summarises the effect
of SRR on the tribofilms formed on the DLC coated balls (mainly when lubricated with O1 and O3).
As can be seen from Table 5, for O1, the DLC ball under sliding/rolling contact mainly consisted of
FeMoO4. For the same oil under pure sliding contact, both MoS2 and FeMoO4were detected on the
DLC surface. This could justify the friction results where lower friction was reported under pure sliding
contact as compared with the sliding/rolling contact. In addition, as the DLC ball under sliding/rolling
contact mainly consisted of FeMoO4, high wear was expected due to enhanced removal of tribofilms
from the DLC ball. Lower wear was reported on the DLC ball under sliding/rolling contact, suggesting
that the wear performance, in some cases, was controlled more by the type of contact than the oil
formulation. For O3 (FF+ZDDP), both Zn 2p and P 2p were observed on the DLC ball under pure
sliding contact while no such compounds were detected on the DLC ball under sliding/rolling contact.
Therefore, higher wear rate was reported for sliding/rolling contact than the pure sliding contact. On
the other hand, for tribofilms formed on the CI discs (see Fig. 15), it can be seen that the MoS2/FeMoO4
ratio varies for the type of contact. In addition, it was found that MoS2/FeMoO4ratio links to friction
Table 5:Effect of SRR on the tribofilms detected on the DLC coated balls using XPS
Sliding/rolling contact Pure sliding contact
O1 Mo 3d (FeMoO4only) Mo 3d (FeMoO4+ MoS2)
O3 - Zn 2p (Zn 2p1/2 + Zn2p3/2) + P 2p
Generally, for most CI discs and DLC balls, there was a considerable variation in the chemical
composition of the tribofilm that formed under both contacts. As a result, film thickness was seen to be
influenced by the change in SRR. From Fig. 19 and Table 6, the film formed on the CI disc lubricated
in O5 (FF+ZDDP+MoDTC) showed that concentrations of elements under pure sliding contact are
significantly lower nearer to the substrate with high concentration of iron as compared to sliding/rolling
contact. However, for DLC balls under both contacts, the depth profiles were fairly similar (i.e. both
having thinner tribofilms). In addition, it can be observed that on cast iron, the thickness depends on
sliding/rolling ratio whereas on DLC it does not.
Table 6:XPS quantification of tribofilms on the CI discs and DLC balls lubricated in O5
Sputter time: 1120s C 1s% Fe 2p% O 1s% Ca 2p% Mo 3d% Zn 2p% P 2p% S 2p%
Disc 50% SRR 20.7 27.2 37.7 5.9 1.0 2.5 2.7 2.0
200% SRR 16.0 64.0 18.7 1.0 0 0 0 0
Ball 50% SRR 98.8 0 1.0 0 0 0 0 0
The present study shows the tribological and tribochemical characteristics of a DLC/uncoated CI
system with MoDTC-type friction modifier under sliding and rolling contacts. The main conclusions
drawn from this work are:
The sliding/rolling ratio affects friction, wear and tribochemistry in CI/DLC systems; pure
sliding enhances MoDTC activation.
Friction coefficient values were observed to vary across the boundary lubrication regime, unlike
most modelling work which assume a constant value for coefficient of friction.
The main MoDTC decomposition products are MoS2and FeMoO4, not MoO3. FeMoO4 was
identified as the reaction species, which is possibly responsible for the high friction.
Tribofilm build-up is related to the sliding/rolling ratio (SRR). For instance, the DLC ball
lubricated in base oil containing MoDTC (i.e. O1) created a film consisted of MoS2 and
FeMoO4 under pure sliding contact while only FeMoO4was detected under sliding/rolling
contact. In addition, for pure sliding contact, Zn 2p and P 2p were observed on the DLC ball
lubricated in the presence of ZDDP additive (i.e. O3 and O5) while no such compounds were
detected on the DLC ball under sliding/rolling contact. All these variations are supported by
the friction and wear results.
MoS2/FeMoO4 ratio played a key role in the tribological performance of the CI discs. MoS2/
FeMoO4for CI discs lubricated in the presence of MoDTC additive (i.e. O1, O4 and O5) was
higher under pure sliding contact as compared with sliding/rolling contact. This correlates with
the obtained friction results.
Regardless of the contact type, no lubricants showed high wear on DLC coating. In addition,
all DLC ballsshowed thinner films compared to CI discs, so the tribofilms were hard to detect
by Raman technique.
The authors would like to thank the Higher Committee for Education Development in Iraq (HCED)
for funding this project and Mr. Sandeep Jhand of Oerlikon Balzers Coating UK Ltd. for supplying the
coatings. Also, the authors wish to thank Total for supplying the lubricants.
 Ahmed Ali M, Xianjun H, Mai L, Bicheng C, Turkson R, Qingping C. Reducing frictional power losses and improving the scuffing resistance in automotive engines using hybrid nanomaterials as nano-lubricant additives. Wear 2016; 364: 270-281.
 Kosarieh S, Morina A, Flemming J, Lainé E, Neville A. Wear mechanisms of hydrogenated DLC in oils containing MoDTC. Tribology Lett 2016;64:4.
 Khaemba DN, Neville A, Morina A. New insights on the decomposition mechanism of Molybdenum DialkyldiThioCarbamate (MoDTC). RSC Advances 2016;6:38637-46.
 Ohara K, Hanyuda K, Kawamura Y, Omura K, Kameda I, Umehara N. Analysis of wear track on DLC coatings after sliding with MoDTC-containing lubricants. Tribology Online 2017;12:110-116.
 Martin J-M, Grossiord C, Le Mogne T, Igarashi J. Transfer films and friction under boundary lubrication. Wear 2000;245:107-15.
 Morina A, Neville A, Priest M, Green JH. ZDDP and MoDTC interactions and their effect on tribological performance – tribofilm characteristics and its evolution. Tribology Lett 2006;24:243-56.
 Yue W, Liu C, Fu Z, Wang C, Huang H, Liu J. Synergistic effects between sulfurized W-DLC coating and MoDTC lubricating additive for improvement of tribological performance. Tribology Int 2013;62:117-23.
 Topolovec-Miklozic K, Lockwood F, Spikes H. Behaviour of boundary lubricating additives on DLC coatings. Wear 2008;265:1893-901.
 Haque T, Morina A, Neville A, Kapadia R, Arrowsmith S. Non-ferrous coating/lubricant interactions in tribological contacts: assessment of tribofilms. Tribology Inter 2007;40:1603-12.
 Haque T, Morina A, Neville A. Tribological performance evaluation of a hydrogenated diamond-like carbon coating in sliding/rolling contact–effect of lubricant additives. J of Engineering Tribol 2011;225:393-405.
 Shinyoshi T, Fuwa Y, Ozaki Y. Wear analysis of DLC coating in oil containing Mo-DTC. SAE Technical Paper 2007, No. 20077103.
 Kosarieh S, Morina A, Lainé E, Flemming J, Neville A. The effect of MoDTC-type friction modifier on the wear performance of a hydrogenated DLC coating. Wear 2013;302:890-8.
 Vengudusamy B, Green JH, Lamb GD, Spikes HA. Behaviour of MoDTC in DLC/DLC and DLC/steel contacts. Tribology Int 2012;54:68-76.
 Sugimoto I. Mechanism on specific wear of DLC film in engine oil with Mo-DTC. Transactions of the Japan society of mechanical engineers 2012;78:213-22.
 Haque T, Morina A, Neville A. Influence of friction modifier and antiwear additives on the tribological performance of a non-hydrogenated DLC coating. Surface and Coatings Tech 2010;204:4001-11.
 Haque T, Morina A, Neville A, Kapadia R, Arrowsmith S. Effect of oil additives on the durability of hydrogenated DLC coating under boundary lubrication conditions. Wear 2009;266:147-57.
 Masuko M, Ono T, Aoki S, Suzuki A, Ito H. Friction and wear characteristics of DLC coatings with different hydrogen content lubricated with several Mo-containing compounds and their related compounds. Tribology Int 2015;82, Part B:350-7.
 De Feo M, De Barros Bouchet MI, Minfray C, Le Mogne T, Meunier F, Yang L. MoDTC lubrication of DLC-involving contacts. Wear 2016;348–349:116-25.
 Vengudusamy B, Grafl A, Novotny-Farkas F, Schöfmann W. Comparison of frictional properties of gear oils in boundary and mixed lubricated rolling–sliding and pure sliding contacts. Tribology Int 2013;62:100-9.
 Brandao JA, Meheux M, Seabra JH, Ville F, Castro M. Traction curves and rheological parameters of fully formulated gear oils. J of Engineering Tribol 2011;225:577-93.
 Ciulli E, Stadler K, Draexl T. The influence of the slide-to-roll ratio on the friction coefficient and film thickness of EHD point contacts under steady state and transient conditions. Tribology Int 2009;42:526-34.
 Meheux M, Minfray C, Ville F, Mogne TL, Lubrecht A, Martin J-M, et al. Influence of slide-to-roll ratio on tribofilm generation. J of Engineering Tribol 2008;222:325-34.
 Shimizu Y, Spikes HA. The influence of slide–roll ratio on ZDDP tribofilm formation. Tribology Lett 2016;64:19.
 Lainé E, Olver A, Lekstrom M, Shollock B, Beveridge T, Hua D. The effect of a friction modifier additive on micropitting. Tribology Tran 2009;52:526-33.
 Jelita Rydel J, Vegter RH, Rivera-Díaz-del-Castillo PEJ. Tribochemistry of bearing steels: A new AFM method to study the material–tribofilm correlation. Tribology Int 2016;98:74-81.
 Ghanbarzadeh A, Parsaeian P, Morina A, Wilson MCT, van Eijk MCP, Nedelcu I. A Semi-deterministic wear model considering the effect of Zinc Dialkyl Dithiophosphate tribofilm. Tribology Lett 2015;61:12.
 Hamrock BJ, Dowson D. Ball bearing lubrication: the elastohydrodynamics of elliptical contacts. 1981.
 Moulder JF, Stickle WF, Sobol PE, Bomben KD. Standard spectra for identification and interpretation of XPS data. Perkin Elmer, Eden Prairie, MN. 1992.
 Vengudusamy B, Mufti RA, Lamb GD, Green JH, Spikes HA. Friction properties of DLC/DLC contacts in base oil. Tribology int 2011;44:922-32.
 Vengudusamy B, Green JH, Lamb GD, Spikes HA. Tribological properties of tribofilms formed from ZDDP in DLC/DLC and DLC/steel contacts. Tribology Int 2011;44:165-74.
 Khaemba DN, Neville A, Morina A. A methodology for Raman characterisation of MoDTC tribofilms and its application in investigating the influence of surface chemistry on friction performance of MoDTC lubricants. Tribology Lett 2015;59:38.
 Mistry K, Morina A, Neville A. Single cam tribometer for evaluating tribological parameters and tribochemistry of DLC coated valve train follower. Tribology-Materials 2012;6:31-7.
 Ofune M, Banks P, Morina A, Neville A. Development of valve train rig for assessment of cam/follower tribochemistry. Tribology Int 2015;93:733-44.
 Grossiord C, Varlot K, Martin J-M, Le Mogne T, Esnouf C, Inoue K. MoS2 single sheet lubrication by molybdenum dithiocarbamate. Tribology int 1998;31:737-43.
 Unnikrishnan R, Jain M, Harinarayan A, Mehta A. Additive–additive interaction: an XPS study of the effect of ZDDP on the AW/EP characteristics of molybdenum based additives. Wear 2002;252:240-9.
 Zhang Z, Li W, Ng T-W, Kang W, Lee C-S, Zhang W. Iron (ii) molybdate (FeMoO4) nanorods as a high-performance anode for lithium ion batteries: structural and chemical evolution upon cycling. J of Materials Chemistry 2015;3:20527-34.
 Zhang Z, Hu C, Hashim M, Chen P, Xiong Y, Zhang C. Synthesis and magnetic property of FeMoO4 nanorods. Materials Science and Engineering 2011;176:756-61.
 Wang Y, He P, Lei W, Dong F, Zhang T. Novel FeMoO4/graphene composites based electrode materials for supercapacitors. Composites Science and Tech 2014;103:16-21.
 Introduction A2 - Niinomi, Mitsuo. Metals for Biomedical Devices: Woodhead Publishing 2010. p. xv-xvii.
 Priest M. Introducion to Tribology and real surfaces. 2011;1:1-76.
 Priest M, Taylor CM. Automobile engine tribology — approaching the surface. Wear 2000;241:193-203.
 Rai Y, Neville A, Morina A. Transient processes of MoS2 tribofilm formation under boundary lubrication. Lubrication Scien 2016;28:449-71.
 Muraki M, Yanagi Y, Sakaguchi K. Synergistic effect on frictional characteristics under rolling-sliding conditions due to a combination of molybdenum dialkyldithiocarbamate and zinc dialkyldithiophosphate. Tribology Int 1997;30:69-75.
 Yamamoto Y, Gondo S. Friction and wear characteristics of molybdenum dithiocarbamate and molybdenum dithiophosphate. Tribology Tran 1989;32:251-7.
 Kasrai M, Cutler J, Gore K, Canning G, Bancroft G, Tan K. The chemistry of antiwear films generated by the combination of ZDDP and MoDTC examined by X-ray absorption spectroscopy. Tribology tran 1998;41:69-77.
 Ratoi M, Niste VB, Alghawel H, Suen YF, Nelson K. The impact of organic friction modifiers on engine oil tribofilms. RSC Advances 2014;4:4278-85.